text: Unsaturated polyesters are condensation polymers formed by the reaction of polyols (also known as polyhydric alcohols), organic compounds with multiple alcohol or hydroxy functional groups, with unsaturated and in some cases saturated dibasic acids. Typical polyols used are glycols including ethylene glycol, propylene glycol, and diethylene glycol; typical acids used are phthalic acid, isophthalic acid, terephthalic acid, and maleic anhydride. Water, a condensation by-product of esterification reactions, is continuously removed by distillation, driving the reaction to completion via Le Chateliers principle. Unsaturated polyesters are generally sold to parts manufacturers as a solution of resin in reactive diluent; styrene is the most common diluent and the industry standard. The diluent allows control over the viscosity of the resin, and is also a participant in the curing reaction. The initially liquid resin is converted to a solid by cross-linking chains. This is done by creating free radicals at unsaturated bonds, which propagate in a chain reaction to other unsaturated bonds in adjacent molecules, linking them in the process. Unsaturation is generally in the form of maleate and fumarate species along the polymer chain. Maleate/fumarate generally does not self-polymerize via radical reactions, but readily reacts with styrene. Maleic anhydride and styrene are known to form alternating copolymers, and are in fact the textbook case of this phenomenon. This is one reason that styrene has been so hard to displace in the market as the industry standard reactive diluent for unsaturated polyester resins, despite increasing efforts to displace the material such as Californias Proposition 65. The initial free radicals are induced by adding a compound that easily decomposes into free radicals. This compound is known as the catalyst within the industry, but initiator is a more appropriate term. Transition metal salts are usually added as a catalyst for the chain-growth crosslinking reaction, and in the industry this type of additive is known as a promoter; the promoter is generally understood to lower the bond dissociation energy of the radical initiator. Cobalt salts are the most common type of promoter used. Common radical initiators used are organic peroxides such as benzoyl peroxide or methyl ethyl ketone peroxide.
  Polyester resins are thermosetting and, as with other resins, cure exothermically. The use of excessive initiator especially with a catalyst present can, therefore, cause charring or even ignition during the curing process. Excessive catalyst may also cause the product to fracture or form a rubbery material.
  Unsaturated polyesters (UPR) are utilized in many different industrially relevant markets, but in general are used as the matrix material for various types of composites. Glass fiber-reinforced composites comprise the largest segment into which UPRs are used and can be processed via SMC, BMC, pultrusion, cured-in-place pipe (known as relining in Europe), filament winding, vacuum molding, spray-up molding, resin transfer molding (RTM). Wind turbine blades also use them as well as many more processes. UPRs are also used in non-reinforced applications with common examples being gel coats, shirt buttons, mine-bolts, , polymer concrete, and  engineered stone/cultured marble.